Disordered misfit [Ca~2~CoO~3~][CoO~2~]~1.62~ structure revisited <i>via</i> a new intrinsic modulation
Muguerra, Hervé; Grebille, Dominique; Bourée, Françoise; Acta Crystallographica Section B 64 (2008) 144–153; doi:10.1107/S0108768108001213

data_2104094
_publ_section_title
;
 Disordered misfit [Ca~2~CoO~3~][CoO~2~]~1.62~ structure revisited
 <i>via</i> a new intrinsic modulation
;
_journal_coeditor_code           SN5060
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              144
_journal_page_last               153
_journal_paper_doi               10.1107/S0108768108001213
_journal_volume                  64
_journal_year                    2008
_chemical_formula_sum            'Ca2 Co2.496 O6.117'
_chemical_formula_weight         325.1
_chemical_name_systematic        ' ?'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   X2/m
_cell_angle_alpha                90
_cell_angle_beta                 98.124
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.8395
_cell_length_b                   4.5531
_cell_length_c                   10.8583
_cell_measurement_temperature    300
_cell_modulation_dimension       2
_cell_subsystems_number          2
_cell_volume                     236.859
_computing_publication_material
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_computing_structure_refinement
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_diffrn_ambient_temperature      293
_diffrn_measurement_device_type  'Bruker Kappa CCD'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0051
_diffrn_reflns_av_sigmaI/netI    0.0454
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_index_m_1_max 1
_diffrn_reflns_limit_index_m_1_min -1
_diffrn_reflns_limit_index_m_2_max 5
_diffrn_reflns_limit_index_m_2_min -1
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4288
_diffrn_reflns_theta_max         44.98
_diffrn_reflns_theta_min         5.80
_exptl_absorpt_coefficient_mu    10.798
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  1.000
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    4.5572
_exptl_crystal_description       plate
_exptl_crystal_F_000             313
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.67
_refine_diff_density_min         -0.71
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.66
_refine_ls_number_parameters     78
_refine_ls_number_reflns         2492
_refine_ls_R_factor_all          0.0629
_refine_ls_R_factor_gt           0.0327
_refine_ls_shift/su_max          0.0158
_refine_ls_shift/su_mean         0.0016
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/\s^2^(F)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0294
_refine_ls_wR_factor_ref         0.0322
_reflns_number_gt                1673
_reflns_number_total             2492
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5060.cif
_cod_data_source_block           (I)
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'None' changed to 'none' according
to '/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'None' changed to 'none'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        236.8586
_cod_database_code               2104094